Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this presentation? Why not share!

- Prestressed concrete by Rajesh Burde 59619 views
- Introduction to prestressed concrete by 9833356555 56600 views
- prestressed concrete by Parag Pal 19680 views
- Prestress loss by Imran Islam 6514 views
- Prestress loss due to friction & an... by Ayaz Malik 4858 views
- Prestressing Concept, Materials and... by সাফকাত অরিন 16722 views

43,907 views

Published on

No Downloads

Total views

43,907

On SlideShare

0

From Embeds

0

Number of Embeds

43

Shares

0

Downloads

2,748

Comments

0

Likes

75

No embeds

No notes for slide

- 1. Prestress Loss
- 2. Introduction • In prestressed concrete applications, most important variable is the prestress. • Prestress does not remain constant (reduces) with time. • Even during prestressing of tendons, and transfer of prestress, there is a drop of prestress from the initially applied stress. • Reduction of prestress is nothing but the loss in prestress.
- 3. • Early attempts to produce prestressed concrete was not successful due to loss of prestress transferred to concrete after few years. • Prestress loss is nothing but the reduction of initial applied prestress to an effective value. • In other words, loss in prestress is the difference between initial prestress and the effective prestress that remains in a member. • Loss of prestress is a great concern since it affects the strength of member and also significantly affects the member’s serviceability including Stresses in Concrete, Cracking, Camber and Deflection. Prestress Loss
- 4. Loss of prestress is classified into two types: 1. Short-Term or Immediate Losses immediate losses occur during prestressing of tendons, and transfer of prestress to concrete member. 2. Long-Term or Time Dependent Losses Time dependent losses occur during service life of structure.
- 5. 1. Immediate Losses include i. Elastic Shortening of Concrete ii. Slip at anchorages immediately after prestressing and iii. Friction between tendon and tendon duct, and wobble Effect 2. Time Dependent Losses include i. Creep and Shrinkage of concrete and ii. Relaxation of prestressing steel
- 6. Prestress Losses Immediate Time Dependent Relaxation Anchorage Slip Elastic Shortening Friction ShrinkageCreep
- 7. Losses in Various Prestressing Systems Type of Loss Pre-tensioning Post-tensioning 1. Elastic Shortening Yes i. No, if all the cables are simultaneously tensioned. ii. If the wires are tensioned in stages loss will exist. 2. Anchorage Slip No Yes 3. Friction Loss No Yes 4. Creep and Shrinkage of Concrete Yes Yes 5. Relaxation of Steel Yes Yes
- 8. Immediate Losses Elastic Shortening of Concrete • In pre-tensioned concrete, when the prestress is transferred to concrete, the member shortens and the prestressing steel also shortens in it. Hence there is a loss of prestress. • In case of post-tensioning, if all the cables are tensioned simultaneously there is no loss since the applied stress is recorded after the elastic shortening has completely occurred. • If the cables are tensioned sequentially, there is loss in a tendon during subsequent stretching of other tendons.
- 9. • Loss of prestress mainly depends on modular ratio and average stress in concrete at the level of steel. • Loss due to elastic shortening is quantified by drop in prestress (Δfp) in a tendon due to change in strain in tendon (Δεp). • The change in strain in tendon is equal to the strain in concrete (εc) at the level of tendon due to prestressing force. • This assumption is due to strain compatibility between concrete and steel. • Strain in concrete at the level of tendon is calculated from the stress in concrete (fc) at the same level due to prestressing force.
- 10. Strain compatibility • Loss due to elastic shortening is quantified by the drop in prestress (∆fp) in a tendon due to change in strain in tendon (∆εp). • Change in strain in tendon is equal to strain in concrete (εc) at the level of tendon due to prestressing force, which is called strain compatibility between concrete and steel. • Strain in concrete at the level of tendon is calculated from the stress in concrete (fc) at the same level due to the prestressing force. • A linear elastic relationship is used to calculate the strain from the stress.
- 11. Elastic Shortening 1. Pre-tensioned Members: When the tendons are cut and the prestressing force is transferred to the member, concrete undergoes immediate shortening due to prestress. 2. Tendon also shortens by same amount, which leads to the loss of prestress.
- 12. Elastic Shortening 1. Post-tensioned Members: If there is only one tendon, there is no loss because the applied prestress is recorded after the elastic shortening of the member. 2. For more than one tendon, if the tendons are stretched sequentially, there is loss in a tendon during subsequent stretching of the other tendons.
- 13. Pre-tensioned Members: operation of pre-tensioning through various stages by animation. Pre-tensioning of a member Prestressing bed Elastic Shortening
- 14. Casting bed Duct jackAnchorage Post-tensioning of a member Post-tensioned Members: complete operation of post-tensioning through various stages by animation Elastic Shortening
- 15. • Linear elastic relationship is used to calculate the strain from the stress. • Quantification of the losses is explained below. Δfp=EpΔεp =Epεc =Ep(fc/Ec) Δfp= mfc • For simplicity, the loss in all the tendons can be calculated based on the stress in concrete at the level of CGS. • This simplification cannot be used when tendons are stretched sequentially in a post-tensioned member.
- 16. • In most Post-tensioning systems when the tendon force is transferred from the jack to the anchoring ends, the friction wedges slip over a small distance. • Anchorage block also moves before it settles on concrete. • Loss of prestress is due to the consequent reduction in the length of the tendon. • Certain quantity of prestress is released due to this slip of wire through the anchorages. – Amount of slip depends on type of wedge and stress in the wire. Anchorage Slip
- 17. • The magnitude of slip can be known from the tests or from the patents of the anchorage system. • Loss of stress is caused by a definite total amount of shortening. • Percentage loss is higher for shorter members. • Due to setting of anchorage block, as the tendon shortens, there develops a reverse friction. • Effect of anchorage slip is present up to a certain length, called the setting length lset.
- 18. • Anchorage loss can be accounted for at the site by over- extending the tendon during prestressing operation by the amount of draw-in before anchoring. • Loss of prestress due to slip can be calculated: s , = Slip of anchorage L= Length of cable A= Cross-sectional area of the cable E = Modulus of Elasticity of steel P = Prestressing Force in the cab sP E A L where le.
- 19. Frictional Loss • In Post-tensioned members, tendons are housed in ducts or sheaths. • If the profile of cable is linear, the loss will be due to straightening or stretching of the cables called Wobble Effect. • If the profile is curved, there will be loss in stress due to friction between tendon and the duct or between the tendons themselves.
- 20. A typical continuous post-tensioned member (Courtesy: VSL International Ltd.) Friction Post-tensioned Members • Friction is generated due to curvature of tendon, and vertical component of the prestressing force. 5
- 21. Variation of prestressing force after stretching Px Friction Post-tensioned Members P0
- 22. • The magnitude of prestressing force, Px at any distance, x from the tensioning end follows an exponential function of the type, o, P = Prestressing force at the jacking end = Coeficient of friction between cable and the duct umulative angle in radian throug kx x oP P e where C h which the tangent to the cable profile has turned between any two points under consideration k = Friction coefficient
- 23. Creep of Concrete • Time-dependent increase of deformation under sustained load. • Due to creep, the prestress in tendons decreases with time. Factors affecting creep and shrinkage of concrete • Age • Applied Stress level • Density of concrete • Cement Content in concrete • Water-Cement Ratio • Relative Humidity and • Temperature Time Dependent Losses
- 24. • For stress in concrete less than one-third of the characteristic strength, the ultimate creep strain (εcr,ult) is found to be proportional to the elastic strain (εel). • The ratio of the ultimate creep strain to the elastic strain is defined as the ultimate creep coefficient or simply creep coefficient, θ. εcr,ult = θεel • IS: 1343 considers only the age of loading of the prestressed concrete structure in calculating the ultimate creep strain.
- 25. • The loss in prestress (Δfp ) due to creep is given as follows. Δfp = Ep εcr, ult =Ep θ εel Since εcr,ult = θ εel Ep is the modulus of the prestressing steel • Curing the concrete adequately and delaying the application of load provide long-term benefits with regards to durability, loss of prestress and deflection. • In special situations detailed calculations may be necessary to monitor creep strain with time. • Specialized literature or standard codes can provide guidelines for such calculations.
- 26. • Following are applicable for calculating the loss of prestress due to creep. • Creep is due to sustained (permanent) loads only. Temporary loads are not considered in calculation of creep. • Since the prestress may vary along the length of the member, an average value of the prestress is considered. • Prestress changes due to creep, which is related to the instantaneous prestress. • To consider this interaction, the calculation of creep can be iterated over small time steps.
- 27. Shrinkage of Concrete • Time-dependent strain measured in an unloaded and unrestrained specimen at constant temperature. • Loss of prestress (Δfp ) due to shrinkage is as follows. Δfp = Ep εsh where Ep is the modulus of prestressing steel. The factors responsible for creep of concrete will have influence on shrinkage of concrete also except the loading conditions.
- 28. • The approximate value of shrinkage strain for design shall be assumed as follows (IS 1383): • For pre-tensioning = 0.0003 • For post-tensioning = Where t = age of concrete at transfer in days. 10 0.002 ( 2)Log t
- 29. Relaxation • Relaxation is the reduction in stress with time at constant strain. – decrease in the stress is due to the fact that some of the initial elastic strain is transformed in to inelastic strain under constant strain. – stress decreases according to the remaining elastic strain.
- 30. Factors effecting Relaxation : • Time • Initial stress • Temperature and • Type of steel. • Relaxation loss can be calculated according to the IS 1343-1980 code.
- 31. Losses in Prestress Notation Geometric Properties 1. Commonly used Notations in prestressed member are • Ac = Area of concrete section = Net c/s area of concrete excluding the area of prestressing steel. • Ap = Area of prestressing steel = Total c/s area of tendons. • A = Area of prestressed member = Gross c/s area of prestressed member = Ac + Ap
- 32. At = Transformed area of prestressed member = Area of member when steel area is replaced by an equivalent area of concrete = Ac + mAp = A + (m – 1)Ap Here, m = the modular ratio = Ep/Ec Ec = short-term elastic modulus of concrete Ep = elastic modulus of steel.
- 33. Areas for prestressed members CGC, CGS and eccentricity of typical prestressed members
- 34. • CGC = Centroid of concrete = Centroid of gravity of section, may lie outside concrete • CGS = Centroid of prestressing steel = Centroid of the tendons. • CGS may lie outside the tendons or the concrete • I = MoI of prestressed member = Second moment of area of gross section about CGC. • It = Moment of inertia of transformed section = Second moment of area of the transformed section about the centroid of the transformed section. • e = Eccentricity of CGS with respect to CGC = Vertical distance between CGC and CGS. If CGS lies below CGC, e will be considered positive and vice versa
- 35. Load Variables • Pi = Initial prestressing force = force applied to tendons by jack. • P0= Prestressing force after immediate losses = Reduced value of prestressing force after elastic shortening, anchorage slip and loss due to friction. • Pe = Effective prestressing force after time-dependent losses = Final prestressing force after the occurrence of creep, shrinkage and relaxation.
- 36. Strain compatibility • Loss due to elastic shortening is quantified by the drop in prestress (∆fp) in a tendon due to change in strain in tendon (∆εp). • Change in strain in tendon is equal to strain in concrete (εc) at the level of tendon due to prestressing force, which is called strain compatibility between concrete and steel. • Strain in concrete at the level of tendon is calculated from the stress in concrete (fc) at the same level due to the prestressing force. • A linear elastic relationship is used to calculate the strain from the stress.
- 37. • The quantification of the losses is explained below • For simplicity, the loss in all the tendons can be calculated based on the stress in concrete at the level of CGS. • This simplification cannot be used when tendons are stretched sequentially in a post-tensioned member.
- 38. Pre-tensioned Axial Members Original length of member at transfer of prestress Length after elastic shortening Pi P0 Elastic Shortening Elastic shortening of a pre-tensioned axial member
- 39. • The stress in concrete due to prestressing force after immediate losses (P0/Ac) can be equated to the stress in transformed section due to the initial prestress (Pi /At). • The transformed area At of the prestressed member can be approximated to the gross area A. • The strain in concrete due to elastic shortening (εc) is the difference between the initial strain in steel (εpi) and the residual strain in steel (εp0). Elastic Shortening
- 40. Pre-tensioned Axial Members Elastic Shortening Pi P0 Length of tendon before stretching εpi εp0 εc Elastic shortening of a pre-tensioned axial member 25
- 41. • The following equation relates the strain variables. εc = εpi - εp0 • The strains can be expressed in terms of the prestressing forces. • Substituting the expressions of the strains • Thus, the stress in concrete due to the prestressing force after immediate losses (P0/Ac) can be equated to the stress in the transformed section due to the initial prestress (Pi /At).
- 42. Problem 1. A prestressed concrete sleeper produced by pre-tensioning method has a rectangular cross-section of 300mm 250 mm (b h). It is prestressed with 9 numbers of straight 7mm diameter wires at 0.8 times the ultimate strength of 1570 N/mm2. Estimate the percentage loss of stress due to elastic shortening of concrete. Consider m = 6.
- 43. Solution a)Approximate solution considering gross section The sectional properties are. • Area of a single wire, Aw = π/4 72 = 38.48 mm2 • Area of total prestressing steel, Ap = 9 38.48 = 346.32 mm2 • Area of concrete section, A = 300 250 = 75 103 mm2 • Moment of inertia of section, I = 300 2503/12 = 3.91 108 mm4 • Distance of centroid of steel area (CGS) from the soffit,
- 44. • Prestressing force, Pi = 0.8 1570 346.32 N = 435 kN • Eccentricity of prestressing force, e = (250/2) – 115.5 = 9.5 mm • The stress diagrams due to Pi are shown. • Since the wires are distributed above and below the CGC, the losses are calculated for the top and bottom wires separately.
- 45. • Stress at level of top wires (y = yt = 125 – 40) • Stress at level of bottom wires (y = yb = 125 – 40),
- 46. • Loss of prestress in top wires = mfcAp (in terms of force) = 6 4.9 (4 38.48) = 4525.25 N • Loss of prestress in bottom wires = 6 6.7 (5 38.48) = 7734.48 N • Total loss of prestress = 4525 + 7735 = 12259.73 N ≈ 12.3 kN • Percentage loss = (12.3 / 435) 100% = 2.83%
- 47. b) Accurate solution considering transformed section. Transformed area of top steel, A1 = (6 – 1) 4 38.48 = 769.6 mm2 Transformed area of bottom steel, A2 = (6 – 1) 5 38.48 = 962.0 mm2 Total area of transformed section, AT = A + A1 + A2 = 75000.0 + 769.6 + 962.0 = 76731.6 mm2 Centroid of the section (CGC) = 124.8 mm from soffit of beam
- 48. • Moment of inertia of transformed section, IT = Ig + A(0.2)2 + A1(210 – 124.8)2 + A2(124.8 – 40)2 = 4.02 108mm4 • Eccentricity of prestressing force, e = 124.8 – 115.5 = 9.3 mm • Stress at the level of bottom wires, • Stress at the level of top wires,
- 49. • Loss of prestress in top wires = 6 4.81 (4 38.48) = 4442 N • Loss of prestress in bottom wires = 6 6.52 (5 38.48) = 7527 N • Total loss = 4442 + 7527 = 11969 N ≈ 12 kN • Percentage loss = (12 / 435) 100% = 2.75 % • It can be observed that the accurate and approximate solutions are close. Hence, the simpler calculations based on A and I is acceptable.
- 50. Pre-tensioned Bending Members • Changes in length and the prestressing force due to elastic shortening of a pre-tensioned bending member. • Due to the effect of self-weight, the stress in concrete varies along length. • To have a conservative estimate of the loss, the maximum stress at the level of CGS at the mid-span is considered.
- 51. 1. Here, Msw is the moment at mid-span due to self-weight. Precise result using At and It in place of A and I, respectively, is not computationally warranted. In the above expression, the eccentricity of the CGS (e) was assumed to be constant. 2. For a large member, the calculation of the loss can be refined by evaluating the strain in concrete at the level of the CGS accurately from the definition of strain. This is demonstrated later for post-tensioned bending members.
- 52. Post-tensioned Axial Members For more than one tendon, if the tendons are stretched sequentially, there is loss in a tendon during subsequent stretching of the other tendons. The loss in each tendon can be calculated in progressive sequence. Else, an approximation can be used to calculate the losses. The loss in the first tendon is evaluated precisely and half of that value is used as an average loss for all the tendons. Here, Pi,j = initial prestressing force in tendon j n = number of tendons The eccentricity of individual tendon is neglected
- 53. Post-tensioned Bending Members The calculation of loss for tendons stretched sequentially, is similar to post-tensioned axial members. For curved profiles, the eccentricity of the CGS and hence, the stress in concrete at the level of CGS vary along the length. An average stress in concrete can be considered. For a parabolic tendon, the average stress (fc,avg) is given by the following equation. Here, fc1 = stress in concrete at the end of the member fc2 = stress in concrete at the mid-span of the member.
- 54. • A more rigorous analysis of the loss can be done by evaluating the strain in concrete at the level of the CGS accurately from the definition of strain. This is demonstrated for a beam with two parabolic tendons post-tensioned sequentially. • In Fig. 7, Tendon B is stretched after Tendon A. The loss in Tendon A due to elastic shortening during tensioning of Tendon B is given as follows. Here, εc is the strain at the level of Tendon A. The component of εc due to pure compression is represented as εc1. The component of εc due to bending is represented as εc2.
- 55. The two components are calculated as follows. Here, A = cross-sectional area of beam PB = prestressing force in Tendon B Ec = modulus of concrete L = length of beam eA(x) = eccentricities of Tendons A, at distance x from left end eB(x) = eccentricities of Tendons B, at distance x from left end I = moment of inertia of beam δL = change in length of beam
- 56. The variations of the eccentricities of the tendons can be expressed as follows. eA1, eA2 = eccentricities of Tendon A at 1 (end) and 2 (centre), respectively. eB1, eB2 = eccentricities of Tendon B at 1 and 2, respectively. Substituting the expressions of the eccentricities in Eqn. (2- 1.12), the second component of the strain is given as follows.
- 57. • Variation of prestressing force after stretching • In the absence of test data, IS:1343 - 1980 provides guidelines for the values of μ and k. • The value of k varies from 0.0015 to 0.0050 per meter length of the tendon depending on the type of tendon. Type of interface μ For steel moving on smooth concrete 0.55 For steel moving on steel fixed to duct 0.30 For steel moving on lead 0.25
- 58. 1. A post-tensioned beam 100 mm 300 mm (b h) spanning over 10 m is stressed by successive tensioning and anchoring of 3 cables A, B, and C respectively as shown in figure. Each cable has cross section area of 200 mm2 and has initial stress of 1200 MPa. If the cables are tensioned from one end, estimate the percentage loss in each cable due to friction at the anchored end. Assume μ = 0.35, k = 0.0015 / m.
- 59. Solution Prestress in each tendon at stretching end = 1200 200 = 240 kN. To know the value of α(L), the equation for a parabolic profile is required. Here, ym = displacement of the CGS at the centre of the beam from the ends L = length of the beam x = distance from the stretching end y = displacement of the CGS at distance x from the ends.
- 60. An expression of α(x) can be derived from the change in slope of the profile. The slope of the profile is given as follows. At x = 0, the slope dy/dx = 4ym/L. The change in slope α(x) is proportional to x. The expression of α(x) can be written in terms of x as α(x) = θ.x, where, θ = 8ym/L2.
- 61. The total subtended angle over the length L is 8ym/L. The prestressing force Px at a distance x is given by Px = P0e–(μα + kx) = P0e–ηx where, ηx = μα + kx For cable A, ym = 0.1 m. For cable B, ym = 0.05 m. For cable C, ym = 0.0 m. For all the cables, L = 10 m. Substituting the values of ym and L
- 62. The maximum loss for all the cables is at x = L = 10, the anchored end. Percentage loss due to friction = (1 – e–ηL) 100% Variation of prestressing forces The loss due to friction can be considerable for long tendons in continuous beams with changes in curvature. The drop in the prestress is higher around the intermediate supports where the curvature is high. The remedy to reduce the loss is to apply the stretching force from both ends of the member in stages.
- 63. Anchorage Slip In a post-tensioned member, when the prestress is transferred to the concrete, the wedges slip through a little distance before they get properly seated in the conical space. The anchorage block also moves before it settles on the concrete. There is loss of prestress due to the consequent reduction in the length of the tendon. The total anchorage slip depends on the type of anchorage system. Typical values of anchorage slip Anchorage System Anchorage Slip (Δs) Freyssinet system 12 - 5mm Φ strands 12 - 8mm Φ strands 4 mm 6 mm Magnel system 8 mm Dywidag system 1 mm
- 64. Due to the setting of the anchorage block, as the tendon shortens, there is a reverse friction. Hence, the effect of anchorage slip is present up to a certain length. Beyond this setting length, the effect is absent. This length is denoted as lset. Variation of prestressing force after anchorage slip
- 65. Force Variation Diagram The magnitude of the prestressing force varies along the length of a post- tensioned member due to friction losses and setting of the anchorage block. The diagram representing the variation of prestressing force is called the force variation diagram. Considering the effect of friction, the magnitude of the prestressing force at a distance x from the stretching end is given as follows. Here, ηx = μα + kx denotes the total effect of friction and wobble. The plot of Px gives the force variation diagram.
- 66. The initial part of the force variation diagram, up to length lset is influenced by the setting of the anchorage block. Let the drop in the prestressing force at the stretching end be ΔP. The determination of ΔP and lset are necessary to plot the force variation diagram including the effect of the setting of the anchorage block. Considering the drop in the prestressing force and the effect of reverse friction, the magnitude of the prestressing force at a distance x from the stretching end is given as follows. Here, η’ for reverse friction is analogous to η for friction and wobble. At the end of the setting length (x = lset), Px = P’x
- 67. Force variation diagram near the stretching end Substituting the expressions of Px and Px’for x = lset Since it is difficult to measure η’ separately, η’ is taken equal to η. The expression of ΔP simplifies to the following. T ∆P = 2P0ηlset
- 68. The following equation relates lset with the anchorage slip Δs. Transposing the terms, Therefore, The term P0η represents the loss of prestress per unit length due to friction.
- 69. The force variation diagram is used when stretching is done from both the ends. The tendons are overstressed to counter the drop due to anchorage slip. The stretching from both the ends can be done simultaneously or in stages. The final force variation is more uniform than the first stretching. Force variation diagrams for stretching in stages
- 70. The force variation diagrams for the various stages are explained. a) The initial tension at the right end is high to compensate for the anchorage slip. It corresponds to about 0.8 fpk initial prestress. The force variation diagram (FVD) is linear. b) After the anchorage slip, the FVD drops near the right end till the length lset.
- 71. c) The initial tension at the left end also corresponds to about 0.8 fpk initial prestress. The FVD is linear up to the centre line of the beam. d) After the anchorage slip, the FVD drops near the left end till the length lset. It is observed that after two stages, the variation of the prestressing force over the length of the beam is less than after the first stage.
- 72. Example A four span continuous bridge girder is post-tensioned with a tendon consisting of twenty strands with fpk = 1860 MPa. Half of the girder is shown in the figure below. The symmetrical tendon is simultaneously stressed up to 75% fpk from both ends and then anchored. The tendon properties are Ap = 2800 mm2, Ep = 195,000 MPa, μ = 0.20, K = 0.0020/m. The anchorage slip Δs = 6 mm. Calculate a) The expected elongation of the tendon after stretching, b) The force variation diagrams along the tendon before and after anchorage.
- 73. Solution Initial force at stretching end 0.75fpk = 1395 MPa P0 = 0.75fpk Ap = 3906 kN The continuous tendon is analysed as segments of parabola. The segments are identified between the points of maximum eccentricity and inflection points. 13.7 13.7 3 3.7 15.2 15.2 3.7
- 74. The inflection points are those where the curvature of the tendon reverses. The different segments are as follows: 1-2, 2-3, 3-4, 4-5, 5-6, 6-7 and 7-8. The following properties of parabolas are used. For segment 1-2, the parabola in the sketch below is used. X e Y L 0 α
- 75. The change in slope from the origin to the end of the parabola is same as the slope at the end of the tendon which is α = 2e/L, where L = length of the segment e = vertical shift from the origin. For segments 2-3 and 3-4 and subsequent pairs of segments, the following property is used.
- 76. For the two parabolic segments joined at the inflection point as shown in the sketch above, the slope at the inflection point α = 2(e1 + e2)/λL. Here, e1 = eccentricities of the CGS at the span e2 = eccentricities of the CGS at the support L = length of the span λL = fractional length between the points of maximum eccentricity The change in slope between a point of maximum eccentricity and inflection point is also equal to α. The change in slope (α) for each segment of the tendon is calculated using the above expressions.
- 77. The value of μα + kx for each segment is calculated using the given values of μ, k and x, the horizontal length of the segment. Since the loss in prestress accrues with each segment, the force at a certain segment is given as follows. The summation Σ is for the segments from the stretching end up to the point in the segment under consideration. Hence, the value of Σ(μα + kx) at the end of each segment is calculated to evaluate the prestressing force at that point (Px, where x denotes the point).
- 78. The force variation diagram before anchorage can be plotted with the above values of Px. A linear variation of the force can be assumed for each segment. Since the stretching is done at both the ends simultaneously, the diagram is symmetric about the central line. a) The expected elongation of the tendon after stretching First the product of the average force and the length of each segment is summed up to the centre line.
- 79. The elongation (Δ) at each stretching end is calculated as follows. b) The force variation diagrams along the tendon before and after anchorage After anchorage, the effect of anchorage slip is present up to the setting length lset. The value of lset due to an anchorage slip Δs = 6 mm is calculated as follows.
- 80. The quantity P0μ is calculated from the loss of prestress per unit length in the first segment. P0μ = (3906 – 3718) kN /13.7 m = 13.7 N/mm. The drop in the prestressing force (Δp) at each stretching end is calculated as follows. Thus the value of the prestressing force at each stretching end after anchorage slip is 3906 – 424 = 3482 kN. The force variation diagram for lset = 15.46 m is altered to show the drop due to anchorage slip. The force variation diagrams before and after anchorage are shown below. Note that the drop of force per unit length is more over the supports due to change in curvature over a small distance.
- 81. Creep of Concrete Creep of concrete is defined as the increase in deformation with time under constant load. Due to the creep of concrete, the prestress in the tendon is reduced with time. The creep of concrete is explained in Section 1.6, Concrete (Part II). Here, the information is summarised. For stress in concrete less than one-third of the characteristic strength, the ultimate creep strain (εcr,ult) is found to be proportional to the elastic strain (εel). The ratio of the ultimate creep strain to the elastic strain is defined as the ultimate creep coefficient or simply creep coefficient θ. The ultimate creep strain is then given as follows.
- 82. IS:1343 - 1980 gives guidelines to estimate the ultimate creep strain in Section 5.2.5. It is a simplified estimate where only one factor has been considered. The factor is age of loading of the prestressed concrete structure. The creep coefficient θ is provided for three values of age of loading. Curing the concrete adequately and delaying the application of load provide long term benefits with regards to durability, loss of prestress and deflection. In special situations detailed calculations may be necessary to monitor creep strain with time. Specialised literature or international codes can provide guidelines for such calculations.
- 83. The loss in prestress (Δfp ) due to creep is given as follows. Δfp = Ep εcr, ult Here, Ep is the modulus of the prestressing steel. The following considerations are applicable for calculating the loss of prestress due to creep. 1) The creep is due to the sustained (permanently applied) loads only. Temporary loads are not considered in the calculation of creep. 2) Since the prestress may vary along the length of the member, an average value of the prestress can be considered. 3) The prestress changes due to creep and the creep is related to the instantaneous prestress. To consider this interaction, the calculation of creep can be iterated over small time steps.
- 84. Shrinkage of Concrete Shrinkage of concrete is defined as the contraction due to loss of moisture. Due to the shrinkage of concrete, the prestress in the tendon is reduced with time. The shrinkage of concrete was explained in details in the Section 1.6, Concrete (Part II). IS:1343 - 1980 gives guidelines to estimate the shrinkage strain in Section 5.2.4. It is a simplified estimate of the ultimate shrinkage strain (εsh). Curing the concrete adequately and delaying the application of load provide long term benefits with regards to durability and loss of prestress. In special situations detailed calculations may be necessary to monitor shrinkage strain with time. Specialised literature or international codes can provide guidelines for such calculations.
- 85. The loss in prestress (Δfp ) due to shrinkage is given as follows. Δfp = Ep εsh Here, Ep is the modulus of the prestressing steel. Relaxation of Steel Relaxation of steel is defined as the decrease in stress with time under constant strain. Due to the relaxation of steel, the prestress in the tendon is reduced with time. The relaxation depends on the type of steel, initial prestress (fpi) and the temperature. To calculate the drop (or loss) in prestress (Δfp), the recommendations of IS:1343 - 1980 can be followed in absence of test data.
- 86. Example A concrete beam of dimension 100 mm 300 mm is post- tensioned with 5 straight wires of 7mm diameter. The average prestress after short-term losses is 0.7fpk = 1200 N/mm2 and the age of loading is given as 28 days. Given that Ep = 200 103 MPa, Ec = 35000 MPa, find out the losses of prestress due to creep, shrinkage and relaxation. Neglect the weight of the beam in the computation of the stresses.
- 87. Solution Area of concrete A = 100 300 = 30000 mm2 Moment of inertia of beam section I = 100 3003 / 12 = 225 106 mm4 Area of prestressing wires, Ap = 5 (π/4) 72 = 192.42 mm2 Prestressing force after short-term losses P0 = Ap.fp0 = 192.4 1200 = 230880 N
- 88. Modular ratio m = Ep / Ec = 2 105 / 35 103 = 5.71 Stress in concrete at the level of CGS = – 7.69 – 2.56 = – 10.25 N/mm2 Loss of prestress due to creep (Δfp)cr = Ep εcr, ult = Ep θεel = Ep θ (fc/Ec) = m θ fc = 5.71 10.25 1.6 = 93.64 N / mm2
- 89. Here, θ = 1.6 for loading at 28 days, from Table 2c-1 (Clause 5.2.5.1, IS:1343 - 1980). Shrinkage strain from Clause 5.2.4.1, IS:1343 - 1980 εsh = 0.0002 / log10(t + 2) = 0.0002 / log10 (28 + 2) = 1.354 10-4 Loss of prestress due to shrinkage (Δfp)sh = Epεsh = 2 105 1.354 10-4 = 27.08 N/mm2 From Table 2c-2 (Table 4, IS:1343 - 1980) Loss of prestress due to relaxation (Δfp)rl = 70.0 N/mm2
- 90. Loss of prestressing force = Δfp Ap Therefore, Loss of prestressing force due to creep =93.64 192.42 = 18018 N Loss of prestressing force due to shrinkage=27.08 192.42 = 5211 N Loss of prestressing force due to relaxation= 70 192.42 = 13469 N Total long-term loss of prestressing force (neglecting the interaction of the losses and prestressing force) = 18018 + 5211 + 13469 = 36698 N Percentage loss of prestress = 36698 / 230880 100% = 15.9 %
- 91. Total Time-dependent Loss The losses of prestress due to creep and shrinkage of concrete and the relaxation of the steel are all time-dependent and inter-related to each other. If the losses are calculated separately and added, the calculated total time-dependent loss is over-estimated. To consider the inter-relationship of the cause and effect, the calculation can be done for discrete time steps. The results at the end of each time step are used for the next time step. This step-by-step procedure was suggested by the Precast / Prestressed Concrete Institute (PCI) committee and is called the General method (Reference: PCI Committee, “Recommendations for Estimating Prestress Losses”, PCI Journal, PCI, Vol. 20, No. 4, July-August 1975, pp. 43-75).
- 92. In the PCI step-by-step procedure, a minimum of four time steps are considered in the service life of a prestres The step-by-step procedure can be implemented by a computer program, where the number of time steps can be increased. There are also approximate methods to calculate lump sum estimates of the total loss. Since these estimates are not given in IS:1343 - 1980, they are not mentioned here. Step Beginning End 1 Pre-tension: Anchorage of steel Post-tension: End of curing Age of prestressing 2 End of Step 1 30 days after prestressing or when subjected to superimposed load 3 End of Step 2 1 year of service 4 End of Step 3 End of service life
- 93. Pretensioning: •In pretensioning system, tendons are first tensioned between rigid anchor blocks cast in the ground. •Concrete is subsequently placed and compacted to the required shape and size. •Pretensioning methods rely on the bond developed between steel and the surrounding concrete. •The tendons should be fully bonded over its entire length. •After the concrete hardens, the tendons are released from the pre- tensioning bed and the prestress is transferred to the concrete.
- 94. Post-tensioning • Concrete units are first cast by incorporating ducts or groves to house the tendons. • When concrete attains sufficient strength, the high tensile wires are tensioned by means of a jack bearing on the end face of the member and the wires are anchored by wedges or nuts. • The forces are transmitted to concrete by means of the end anchorages and also when the cable is curved, through the radial pressure between the cable and the duct. • The space between the tendons and the duct is generally grouted after the tensioning operation.
- 95. + + = e [g+q] P + Direct Stress Bending Stress Resultant Stress P
- 96. Pressure line or Thrust line • Combined action of prestressing force and the externally applied load results in a distribution of concrete stresses that can be resolved into a single force. • The resultant force will occupy different locations in the cross-section at different locations along the beam. • The line joining the locus of points of the resultant force in any structure is termed as the “Pressure or Thrust line”. • The concept of pressure line is very useful in understanding the load carrying mechanism of a prestressed concrete section. • The location of the pressure line depends upon the magnitude and direction of the moments applied at the cross-section and the magnitude and distribution of stress due to the prestressing force.
- 97. Load Balancing Concept • The cable profile is selected in PSC members such that the transverse component of the cable force balances the given type of external loads. • In general, the requirement will be satisfied, if the cable profile coincides with the shape of the BMD resulting from external loads. Reaction of cable curved Tendon and Beam Straight Tendon Bent Tendon

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment